We present a combined approach to photo-assisted degradation processes, in which a catalyst, H2O2 and UV irradiation are used together to enhance the oxidation of Rhodamine B (RB). The heterogeneous photocatalyst was made by the process of adsorption of copper phthalocyanine tetrasulfonic acid (CuPC) onto purified spongin-based Hippospongia communis marine sponge skeleton (HcS). The product obtained, CuPC-HcS, was investigated by a variety of spectroscopic (carbon-13 nuclear magnetic resonance 13C NMR, Fourier transform infrared spectroscopy FTIR, energy-dispersive X-ray spectroscopy EDS) and microscopic techniques (scanning electron microscopy SEM, fluorescent and optical microscopy), as well as thermal analysis. The study confirms the stable combination of the adsorbent and adsorbate. For a 10 mg/L RB solution, the percentage degradation reached 95% using CuPC-HcS as a heterocatalyst. The mechanism of RB removal involves adsorption and photodegradation simultaneously.
Phthalocyanines are macrocyclic, aromatic compounds based on the porphyrin structure, in which four indole rings are connected by azomethine bridges. Because of their specific chemical structure, they exhibit unique properties, which make them suitable for a wide range of applications. Metalphthalocyanines possess high chemical and thermal stability, high reactivity, redox properties and high molar absorption coefficients [1–4]. Moreover, the type, position, and number of substituents and the central atom can change the physical and chemical properties of a phthalocyanine molecule .
Metalphthalocyanines are used as sensors [2,5], photosensitizers in photodynamic therapy and solar cells (DSSC)  and dyes (photochromic substances, fluorescent probes in sensing or in vitro imaging applications). They are semiconductive and light-absorbing electron donor compounds, and can serve in electronic and optoelectronic devices , photovoltaic cells, electrode modifications [7,8], liquid crystals  and data storage systems [10,11]. Phthalocyanines are also commonly used as catalysts, in organic synthesis , degradation of organic pollutants (e.g. 2,4-D acid , synthetic dyes [14,15]), and oxidation of harmful and undesirable compounds (e.g. bisphenol A , phenols , thiols [18,19]).
Metalphthalocyanines exhibit high catalytic activity (in a so-called biomimetic catalytic system) even in ambient conditions ; in addition they are relatively easy to synthesize and commercially available . However, one limitation of these compounds is that they are inconvenient to use, since they are generally available only as powder, in solution (which hinders their separation from the solution and catalyst recycling) or in the form of thin film [22–24]. Moreover, some molecules are prone to aggregation, which greatly decreases the number of active sites for catalysis . A better strategy for their practical use might be to attach them to a suitable support material. Adsorption of metalphthalocyanines on a solid support is an effective way to remedy the drawbacks of the homogeneous catalyst and enable the creation of a heterogeneous system (possibility of reutilization, increase in the surface area of the catalyst). Adsorbents used to date include zeolites , silica , TiO2 , carbon materials [19,28], polymers  and fabrics .
In the present work we decided to use 3-dimensional fibrous proteinaceous skeletons (built from a specific protein – spongin) of marine demosponge origin. In comparison with traditional supports, this material does not have to be synthesized, and the process of adsorption is fast, facile and takes place in mild conditions. Mediterranean Hippospongia communis sponge possess a fibrous, anastomosing, spatial, reticular structure. The structure of spongin is multileveled - single fibers, composed of microfibers, combine into a complex hierarchical network. Spongin fibers may range in thickness from a few mm to about 10-15 mm. The combination of this renewable material with a relative large internal surface area (between 25 and 34 m2 for a 3- to 4-gram skeleton ) with copper phthalocyanine enable the production of the heterocatalyst.
Sponges (phylum Porifera) are one of the phylogenetically oldest multicellular organisms, which evolution dates back to 600 million years ago. They are aquatic animals, currently described in four classes: Demospongiae, Calcarea, Hexactinellida and Homoscleromorpha . Demosponges skeletons are fibrous and contain species dependent chitin, or spongin as main organic constituents. Spongin contains both collagen- and keratin-like structural proteins that are responsible for the rigidity of the sponge skeleton [31,32]. Because of their unique spatial structure and properties (e.g. high thermal stability) spongin-based skeletons of diverse demosponges are currently the subjects of numerous studies related to tissue engineering [33,34], as well as to Extreme Biomimetics [35,36]. Due to diverse marine ranching techniques used for the cultivation of spongin-based demosponges, spongin is the renewable source (which affect their relatively low price) of proteinaceous scaffolds with good perspective for practical applications.
In the present work, for the first time, copper phthalocyanine tetrasulfonic salt (CuPC) was successfully adsorbed onto purified marine bath sponge skeleton from the species Hippospongia communis. In addition, we investigated the photocatalytic properties of the resulting systems for organic pollution degradation, using the synthetic dye Rhodamine B as the target compound. Although UV light-assisted photocatalytic degradation of RB has been reported in the literature, the removal of RB using marine sponge skeleton has not previously been studied.
Specimens of Hippospongia communis demosponge were collected on the Mediterranean coast in Tunisia and supplied by INTIB GmbH (Germany). Pieces of selected sponges were prepared by washing with sea water, followed by drying and rinsing again with fresh water five times. To remove contaminants (such as CaCO3) the pieces were immersed in a 3M HCl solution for 72 h at room temperature and finally washed with distillated water up to a neutral level of pH. Copper phthalocyanine- 3,4ʹ,4ʺ,4ʺʹ-tetrasulfonic acid tetrasodium salt (CuPC) and Rhodamine B (RB) were purchased from Sigma Aldrich (Germany). Other chemicals were of reagent grade and used as supplied.
2.2 Adsorption and desorption process
To evaluate the adsorption properties of the purified marine sponge skeleton with respect to CuPC, a series of adsorption experiments were performed. Typically, sponge pieces of 0.1 g were shaken with 25 mL of experimental solutions of desired concentrations (for kinetic studies 50, 100 and 200 mg/L) at pH=2. After predetermined time intervals, the adsorbed quantity (mg/g) of CuPC at time t, qt, was calculated from the following equations:
where C0 and Ct are the concentrations of the dye in the solution before and after sorption (mg/L), V is the volume of the solution (L), and m is the mass of sorbent (g).
Initial dye concentrations for kinetic studies ranged from 50 to 200 mg/L (pH=2).
In order to study the adsorption isotherm, 0.1 g of marine sponge skeleton was kept in contact with 25 mL of dye solution at different concentrations (50, 100, 200, 300, 400 and 500 mg/L) at pH=2 for 240 min with constant shaking at ambient temperature.
To define the most suitable condition for adsorption the effect of several parameters on this process was checked. For studying the effect of solution pH on dye adsorption, experiments at different pH values (ranging from 2 to 11) were performed for an initial dye concentration of 100 mg/L. To observe the effect of NaCl on dye adsorption, different amounts of salt (in concentrations from 0.01 to 1.0 M) were used with 100 mg/L of CuPC solution at initial pH. An adsorbent dose of 0.1 g, contact time 60 min, initial pH and no NaCl were used for all of the above experiments.
The desorption efficiencies of CuPC from the sorbent were measured after the adsorption experiments were completed (100 mg/L, pH=2, contact time 120 min). These studies were carried out in water at ambient temperature and in water with ultrasound at 40, 50 and 60 °C, for 300 min. A standard technique was used to determine the dye concentration using a UV-Vis spectrophotometer (Jasco V750, Japan).
Cross polarization solid state magic angle spinning nuclear magnetic resonance (13C CP MAS NMR) spectra were obtained at a 13C frequency of 100.63 MHz on a DSX spectrometer (Bruker, Germany). Samples were packed in a 4-mm-diameter cylindrical zirconia rotor and spun at 8 kHz.
To confirm the effectiveness of the adsorption process, Fourier transform infrared spectroscopy (FTIR) was performed, using a Vertex 70 spectrometer (Bruker, Germany). The samples were analyzed in the form of tablets, produced by pressing a mixture of anhydrous KBr (ca. 0.25 g) and 1 mg of the tested substance in a special steel ring under a pressure of 10 MPa. The investigation was performed over a wavenumber range of 4000–400 cm–1 at a resolution of 0.5 cm–1.
Energy dispersive spectroscopy (EDS) measurements were carried out using a PTG Prism Si(Li) (Princeton Gamma Tech., USA) energy-dispersive X-ray spectrometer. Before the analysis, samples were placed on the ground with a carbon paste or tape. The presence of carbon materials is needed to create a conductive layer which provides the delivery of electric charge from the sample.
Thermogravimetric (TG) analysis of samples of products was carried out with a Jupiter STA 449F3 analyzer (Netzsch, Germany) with an Al2O3 crucible. The measurements were performed in a nitrogen atmosphere at a heating rate of 10 °C-min4, over a temperature range of 25–1000 °C, with an initial sample weight of approximately 5 mg.
Samples of H. communis sponge skeleton before and after the adsorption process were observed using a Keyence BZ-9000 (Japan) microscope in light as well as in fluorescent microscopy mode.
Photographs were also taken using an EVO40 scanning electron microscope (Zeiss, Germany) to obtain data on surface morphology and structure.
2.4 Photocatalytic activity
The catalytic reactions were carried out by adding 20 mg of a photocatalyst (sponge skeleton with CuPC, obtained after adsorption from 400 mg/L solution at pH=2 for 4 h) to a glass tube reactor containing 30 mL of 10 mg/L RB solution. The reaction mixture was continuously shaken by a magnetic stirrer. Photochemical degradation was carried out in a UV-reactor system (UV-RS-2, Heareus, Germany), equipped with a 150 W medium-pressure mercury lamp, surrounded by a water-cooling quartz jacket to cool the lamp. At given intervals of illumination, 1 mL of the RB solution was taken and decreases in the concentration of dye were analyzed by a Jasco V750 UV-Vis spectrophotometer (halogen lamp) at λ=554 nm. The efficiency of degradation catalyzed by marine sponge skeleton–CuPC hybrid material (CuPC-HcS) was evaluated by means of the RB degradation ratio, given by the following formula:
where C and C0 represent the time-dependent concentration and the initial concentration (determined from the calibration curve), respectively. All the experiments were performed three times.
3 Results and discussion
3.1 Adsorption and desorption process
3.1.1 Influence of time and initial dye concentration
The influence of time and initial dye concentration was investigated in optimal experimental conditions, with controlled pH, ionic strength and temperature.
The changes in the quantity of dye adsorbed (qt) are significant in the first minutes of the process; then with time they become smaller until equilibrium is reached (Fig. 1). Equilibrium is reached faster for a CuPC solution with lower initial concentration (60 min for dye concentrations of 50 and 100 mg/L and 300 min for 200 mg/L). The adsorption efficiency reaches 100% for CuPC (independently of initial dye concentration). The quantity of dye adsorbed on the support increases when the initial dye concentration increases, which is a typical situation explained by the influence of mass gradient and the action of mass transfer driving forces .
3.1.2 Influence of pH and ionic strength
The next stage of the study involved examination of different adsorption conditions (pH and ionic strength) and their influence on process efficiency. In each case only one parameter was changed, while all other variables (time, initial concentration) were kept constant.
In the case of CuPC the greatest effect on the quantity of dye adsorbed (qt) resulted from the pH of the dye solution. Under basic and weak acidic conditions, the values obtained for the efficiency of the process are similar, at around 60%, but a considerable change is noted at pH=2, where the efficiency increases to 98%. In these conditions ionization of functional groups of the amino acids building spongin (NH2→NH3+) takes place, which results in their mutual attraction (in contrast to the repulsive forces in an alkaline environment). These results suggest that the driving force of the adsorption may be electrostatic interactions . The dye molecules can reach the surface of the H. communis sponge skeleton, where they can interact via hydrogen bonding. The pH=2 was chosen as the best condition for all further adsorption process.
The adsorption of dye on the marine sponge skeleton was positively affected by the presence of NaCl. The best results were obtained in the presence of 1M NaCl in the dye solution. The addition of salt ions affects the interaction between adsorbent and adsorbate, due to the increase in ionic strength, a decrease in the thickness of the electrical double layer surrounding particles in solution is observed. Both the repulsive and attractive interactions will be weaker, which increases or decreases the efficiency of the process, depending on which of these interactions occur between the particles in solution . Furthermore, the addition of NaCl increases the value of van der Waals forces, ionion and ion-dipole forces, which positively influences the effectiveness of the adsorption process .
Desorption tests were performed to evaluate the strength of the connection between H. communis skeleton and dye. It was observed that shaking with water at room temperature and ultrasound-assisted washing at 30, 50 and 60 °C, causes only slight elution of the previously adsorbed CuPC (5%).
3.2 Kinetics and isotherms of adsorption
To determine the rate and mechanism of the process of adsorption, pseudo-first-order and pseudo-second-order kinetic models were fitted to the experimental data. These models present the correlations between changes in the concentration of adsorbate as a function of the time for which the adsorption process is continued, until equilibrium is reached.
As can be seen from Fig. 2a and Table 1, the pseudo-second-order model better describes the experimental data. In spite of the relatively high values of the correlation coefficients for the pseudo-first-order model, it cannot be considered useful because of the large differences between the experimental and calculated sorption capacities.
|Parameters||Units||50 mg/L||100 mg/L||200 mg/L|
where: k1 and k2 - rate constants of the pseudo-first-order and pseudo-second-order models respectively, r - correlation coefficient, qe,exp and qe,cel - experimental and calculated adsorption capacity at equilibrium, h - initial adsorption rate.
where Ce denotes the equilibrium concentration of the dye solution (mg/L), qe is the quantity of dye adsorbed at equilibrium (mg/g), Kf (mg/g) and n are the Freundlich constants. The values of Kf and n can be determined from the intercept and gradient of the plot of log(qe) against log(Ce).
where Ce is the equilibrium concentration of the dye solution (mg/L), qm is the maximum adsorption capacity (mg/g), and b is the Langmuir constant (L/mg), which is calculated from the intercept and downward linear slope of the graphs of Ce/qe and Ce.
A graph of qe against Ce for the adsorption isotherms of CuPC on marine sponge skeletons is shown in Fig. 2b.
Analysis of the isotherm parameters obtained for the Freundlich and Langmuir models indicates that the adsorption of CuPC on marine sponge skeleton is a complex process. The calculated correlation coefficients (r2) are similar, 0.917 for Langmuir and 0.957 for Freundlich model. H. communis sponge skeleton has a relatively high maximum adsorption capacity (qm) for copper phthalocyanine (83.36 mg/g). The parameter n in the Freundlich isotherm model is equal to 3.46 (n>1). A value of 1/n below one indicates normal adsorption, while if 1/n is above one it indicates cooperative adsorption; additionally, the smaller the value of 1/n, the greater the heterogeneity of the adsorbate.
3.3 13C CP/MAS NMR
Figure 3 shows the results of 13C MAS NMR analysis.
Marine sponge spongin has an inexact chemical structure, but tentative assignments of some of the unknown components can be made. Signals in the range 17.7–69.6 ppm suggest the presence of alkyl carbons (RCH2, RCH3), carbons bonded to oxygen (RCH2O–) (above 50 ppm), nitrogen (RCH2NH2), as well as halogen atoms (C–Cl, C–Br, C–I, C–SR) (below 50 ppm). The peaks above 115 ppm can be assigned to RHC=CH and aromatic carbons, and those at 170.0 and 172.1 to C=O in acids and esters respectively.
As stated in [45,46] the signals observed in the CuPC spectrum can be ascribed to C1 (141.3 ppm), C2 (128.4 ppm), C3 (126.2 ppm) and C4 (138.4 ppm) incorporated in the carbon structure. Comparing the carbon NMR spectra of marine sponge skeleton with copper phthalocyanine (Fig. 3b and 3c) with the spectra of a sample of H. communis (Fig. 3d) and CuPC (Fig. 3a), it is evident that the CuPC macrocycle carbons appear as a series of lines in the range 120–130 ppm in the spectra of samples 1 and 2. Furthermore a slight downfield shift movement of the alkyl carbons of the marine sponge skeleton provides additional characterization of the new materials.
The results of FTIR analysis of marine sponge skeleton prior to and after the adsorption process, and of CuPC, are presented in Fig. 4. The detailed characterization of the H. communis skeleton can be found in our previous work . Many differences appear in the spectrum after dye adsorption, especially below 1200 cm–1, compared with the H. communis spectrum. The most important changes related to the stretching asymmetric vibrations of sulfonic acid salts (–SO3−M+) occurring in the wavenumber range 1250–1140 cm–1 in the form of a broad band divided into a few smaller peaks. The position of these signals is strongly dependent on the nature of the metal ion which is incorporated in the –SO3− group, as reported earlier in . The effect of the type of carbon atom (alkyl or aryl) connected to the sulfur atom on the position and shape of these bands is much less significant. Additionally, it should be noted that an additional signal is present in the spectrum of the CuPC-HcS material at 1026 cm–1. This peak is shifted in comparison with the spectrum of the crude dye (maximum at 1032 cm–1), which proves the effective adsorption of the CuPC . Furthermore, a signal confirming deposition of the dye, absent from the spectrum of H. communis, is present at 1339 cm–1, generated by stretching vibrations of the −C=C−N− bonds in indole rings. In the CuPC-HcS spectrum a series of specific bands are observed at wavenumbers 746, 699, 649 and 599 cm–1, which come from the interactions between Cu and its ligands. Additionally the broad and strong signal in the range 3500–3200 cm–1 in this spectrum can be attributed to stretching vibrations of −OH and −NH groups. This signal has a different shape than in the spectra of the materials before the adsorption process. A slight shift in the maximum of this band suggests the formation of chemical bonds (hydrogen bonds) between the sponge and the phthalocyanine dye.
Table 2 shows the results of energy dispersive spectroscopy (EDS) analysis for H. communis skeleton, copper phthalocyanine and selected samples obtained after the adsorption process (sample 1: pH=2, 120 min, 500 mg/L; sample 2: pH=2, 120 min, 400 mg/L; sample 3: pH=2, 120 min, 300 mg/L).
|Element content (wt.%)||H. communis||CuPC||SAMPLE 1||SAMPLE 2||SAMPLE 3|
The H. communis skeleton, as well as CuPC, consists mainly of carbon and nitrogen, but these elements are not shown in the table. The data given in Table 2 indicate the presence of oxygen, sodium, aluminum, silica, sulfur, chlorine, iodine and calcium. These elements are naturally occurring in the H. communis skeleton. The occurrence of elements at low concentration (I, Cl, S, Ca, Al) is in accordance with previously published reports [49,50] and implies that some of the spongin-built amino acids may contain heteroatoms. However, the chemical composition of spongin has not yet been precisely determined. In the measured region of the samples after the adsorption process we observe the presence of Cu atoms, which provides direct confirmation of the effectiveness of the adsorption process.
Figure 5 shows TG curves for the H. communis skeleton (HcS), copper phthalocyanine tetrasulfonic acid (CuPC), and the obtained hybrid material (CuPC-HcS).
Thermal decomposition of sulfonated phthalocyanine proceeds in a few steps. The first slight mass loss (about 10%) is probably connected with loss of moisture (up to 200°C). Between 430 and 530°C, the material had lost another 10% of its mass, the loss and fragmentation of substituent units of the environment of the phthalocyanine molecule occurs . Studies  have found that in the range 530–730 °C rupture of macroheterocycles takes place. The residues remaining after thermal decomposition correspond to the metal (in this case copper) oxides .
The rate of degradation of marine sponge skeleton is higher than that of CuPC. This is a result of the thermal decomposition of spongin. As observed on the TG curve, the obtained hybrid material undergoes two stages of mass loss: the first below 120°C, and the second starting at 230°C to reach a plateau near 560°C. These can be attributed respectively to water loss and degradation of the protein-like support. The total mass loss in the case of HcS alone (73%) is higher than in the case of CuPC-HcS (67%).
3.7 Microscopy observations
The images from light, fluorescent and SEM microscopes of samples before and after the adsorption process are presented below. The adsorption process conditions were as follows: pH=2, 120 min, 400 mg/L.
It is reported in the literature  that autofluorescence is usually a superposition of fluorescence from a mixture of individual fluorescent molecules (fluorophores). Fluorophores such as amino acids (e.g. tyrosine) emit fluorescent light due to heterocyclic aromatic rings (such structures are also present in spongin) or conjugated double bonds within their molecular structures. H. communis fibers exhibit photoluminescence, in blue, green as well as red light. A decrease in fluorescent intensity is clearly visible especially in the case of red light, which provides indirect confirmation that the adsorption is a chemical process (Fig. 6).
Fluorescence of some other Demospongiae species have been reported, but the measurements were made in situ and fluorescence was caused by symbiotic or commensal algae or cyanobacteria on the sponge skeletons .
Although the photographs from the light microscope imply that the spongin fibers are entirely covered, the SEM images reveal that there is not a homogenous layer of CuPC on the fibers. The bundle of fibrils forming the spongin fibers is still visible (Fig. 7).
Electro- and sonochemical reactions or oxidation by ozone are sometimes used to remove Rhodamine B, but the most frequently used methods are adsorption and photodegradation. Very often porphyrin or phthalocyanines areusedascatalystsinthese processes. The photodegradation process is very often enhanced by using an external oxidant, e.g. hydrogen peroxide [56–58].
To investigate the catalytic performance of the prepared heterogeneous catalysts and the influence of various factors on RB elimination, a number of experiments were carried out. We monitored the photodegradation of RB molecules under UV irradiation (190–300 nm) by measuring the UV-Vis spectra of filtrate solutions. H. communis skeleton is capable of adsorbing dyes, as was demonstrated above, thus it is possible that RB will also be adsorbed on this support. According to the results presented in Fig. 8 (curve b), the adsorption of Rhodamine B on the sponge skeleton does indeed take place, and the efficiency of the process reaches 32%. This parameter is even higher (65%) when CuPC+HcS (obtained from dye solution at concentration of 400 mg/L at pH=2 for 4 h) is used as the adsorbent (Fig. 8, curve d). A possible explanation of this effect (that sponge with previously adsorbed dye adsorbs better than the pure spongin) may be that functional groups of CuPC interact with the cationic dye RB by electrostatic interaction.
UV irradiation itself does not have any influence on RB degradation (Fig. 8, curve a). The effect is observed in the presence of H2O2 (62%; Fig. 8, curve c) and CuPC-HcS (75%; Fig. 8, curve e). As expected, the addition of H2O2 improves the efficiency of decolorization, but is not effective enough to oxidize RB if used alone. Up to 95% of the RB was photodegraded when both CuPC-HcS as catalyst and H2O2 as oxidant were present, and the concentration of RB decreased quickly within 1 h (Fig. 8, curve f).
A possible mechanism of dye degradation under irradiation is proposed based on the reported mechanism involving both H2O2 and CuPC. The action of metalphthalocyanine causes several successive reactions with the excited singlet and triplet form of metalphthalocyanine and oxygen, which finally decompose the dye [13,59]:
Moreover CuPC can act as a catalyst and activate the H2O2 molecules:
As stated in  there is a possibility for copper to exist as Cu(III) in a complex with porphyrin. The produced hydroxyl radical oxidizes RB:
The hydroxyl radical generated from hydrogen peroxide reacts with RB (equation IX) and gives an intermediate product, which decomposes into the final oxidation product (X). Furthermore, irradiation with UV light causes the excitation of rhodamine (XI). The produced RB* reacts with oxygen, and as a result the cationic radical form of the dye (RB+•) and superoxide (O2−•) are formed (XII). Subsequently, via further reaction with oxygen, the dye is degraded [14,63]. The oxidation products of RB are thoroughly investigated and described in [64,65].
Zhang et al. investigated the photocatalytic activities of 2,9,16,23-tetra-nitrophthalocyanine copper(II) (TNCuPc)/TiO2 composites with respect to Rhodamine B degradation. The TiO2 nanofibers function as an electron trap for the excited surface-adsorbed TNCuPc dye. The trapped electron subsequently induces the generation of active oxygen species, which degrade Rhodamine B with high efficiency, up to almost 90% . Shang et al. also showed the effect of copper phthalocyanine tetrasulfonic acid-sensitized TiO2 on Rhodamine B degradation . The authors achieved total degradation efficiency, although the process required the hydrothermal synthesis of the catalyst, which increases operational costs in comparison with the fast and facile adsorption technique described in the present work. The authors confirmed that the presence of copper phthalocyanine considerably enhanced the photocatalytic activity of titanium dioxide. Another study on the synthesis of a titanium dioxide–copper phthalocyanine hybrid composite and its use in decomposition of Rhodamine B under UV irradiation was published by Mekprasart et al. The system obtained cause decomposition of over 80% of the dye. The significant improvement in photocatalytic activity in the case of the hybrid composite may be linked to the enhancement of optical absorption and the inhibition of electron–hole recombination caused by the presence of CuPC in the TiO2 matrix .
In the cited works, copper phthalocyanines were immobilized on TiO2, which itself is photocatalytically active. Thus the results obtained represent a combination of the photocatalytic properties of both materials. By contrast, in our study we used a biopolymer matrix which is inert under UV irradiation. Hence the presented results relate only to the activity of the phthalocyanine in the dye decomposition process.
In this study a copper phthalocyanine–H. communis marine sponge skeleton hybrid material (CuPC-HcS) was produced with high efficiency by an adsorption process. Adsorption is a fast and simple way to obtain such systems, and does not require sophisticated equipment. The highest efficiencies were obtained from an acidic solution, which suggests that electrostatic interactions occur between the dyes and support. Furthermore, results from spectroscopic analysis indicate the formation of hydrogen bonds. The product was used in the photobleaching of Rhodamine B solution. In these reactions CuPC-HcS serves as a photosensitizer and H2O2 as an external oxidant. Adsorption and simultaneous catalytic oxidation are responsible for RB removal, and all of the analyses performed suggest that it is highly desirable to integrate the advantages of both high adsorption capacity and photocatalytic activity into a single compound.
This work was financially supported by Poznan University of Technology research grant no. 03/32/DSMK/0610 (Poland) as well as by DFG Grant HE 394/3-2 (Germany).
 Singh V. K., Kanaparthi R. K., Giribabu L., Emerging molecular design strategies of unsymmetrical phthalocyanines for dye-sensitized solar cell applications, RSC Adv., 2014, 4, 6970–698410.1039/c3ra45170dSearch in Google Scholar
 Asedegbega-Nieto E., Pérez-Cadenas M., Carter J., Anderson J. A., Guerrero-Ruiz A., Preparation and surface functionalization of MWCNTs: study of the composite materials produced by the interaction with an iron phthalocyanine complex, Nanoscale Res. Lett., 2011, 6, 1–410.1186/1556-276X-6-353Search in Google Scholar
 Harbeck M., Erbahar D. D., Gürol I., Musluoğlu E., Ahsen V., Öztürk Z. Z., Phthalocyanines as sensitive coatings for QCM sensors operating in liquids for the detection of organic compounds, Sensors Actuators B Chem., 2010, 150, 346–35410.1016/j.snb.2010.06.062Search in Google Scholar
 Wróbel D., Dudkowiak A., Porphyrins and phthalocyanines – Functional molecular materials for optoelectronics and medicine, Mol. Cryst. Liq. Cryst., 2006, 448, 617–64010.1080/15421400500377354Search in Google Scholar
 Peeters K., De Wael K., Bogaert D., Adriaens A., The electrochemical detection of 4-chlorophenol at gold electrodes modified with different phthalocyanines, Sensors Actuators, B Chem., 2008, 128, 494–49910.1016/j.snb.2007.07.039Search in Google Scholar
 Wael K., Peeters K., Bogaert D., Buschop H., Vincze L., Adriaens A., Electrochemical and spectroscopic characterization of a gold phthalocyanine, J. Electroanal. Chem., 2007, 603, 212–21810.1016/j.jelechem.2007.02.010Search in Google Scholar
 Lee W., Yuk S. B., Choi J., Jung D. H., Choi S. H., Park J., Kim, J. P., Synthesis and characterization of solubility enhanced metal-free phthalocyanines for liquid crystal display black matrix of low dielectric constant, Dye. Pigment., 2012, 92, 942–94810.1016/j.dyepig.2011.08.001Search in Google Scholar
 Majumdar H. S., Bandyopadhyay A., Pal A. J., Data-storage devices based on layer-by-layer self-assembled films of a phthalocyanine derivative, Org. Electron., 2003, 4, 39–4410.1016/S1566-1199(03)00007-7Search in Google Scholar
 Lian K., Li R., Wang H., Zhang J., Gamota D., Printed flexible memory devices using copper phthalocyanine, Mater. Sci. Eng. B-Advanced Funct., Solid-State Mater., 2010, 167, 12–1610.1016/j.mseb.2010.01.020Search in Google Scholar
 Shinu V. S., Pramitha P., Bahulayan D., A novel highly stereoselective multi-component synthesis of N-substituted β-amino ketone derivatives using copper(II) phthalocyanine as reusable catalyst, Tetrahedron Lett., 2011, 52, 3110–311510.1016/j.tetlet.2011.04.016Search in Google Scholar
 DeOliveira E., Neri C. R., Ribeiro A. O., Garcia V. S., Costa L. L., Moura A. O., Prado A. G. S., Serra O. A., Iamamoto Y., Hexagonal mesoporous silica modified with copper phthalocyanine as a photocatalyst for pesticide 2,4-dichlorophenoxiacetic acid degradation, J. Colloid Interface Sci., 2008, 323, 98–10410.1016/j.jcis.2008.04.025Search in Google Scholar
 Sharma R. K., Gulati S., Pandey A., Adholeya A., Novel, efficient and recyclable silica based organic–inorganic hybrid nickel catalyst for degradation of dye pollutants in a newly designed chemical reactor, Appl. Catal. B Environ., 2012, 125, 247–25810.1016/j.apcatb.2012.05.046Search in Google Scholar
 Zhang M., Shao C., Guo Z., Zhang Z., Mu J., Zhang P., Cao T., Liu Y., Highly efficient decomposition of organic dye by aqueous-solid phase transfer and in situ photocatalysis using hierarchical copper phthalocyanine hollow spheres, ACS Appl. Mater. Interfaces, 2011, 3, 2573–257810.1021/am200412tSearch in Google Scholar
 Sasai R., Watanabe R., Yamada T., Preparation and characterization of titania- and organo-pillared clay hybrid photocatalysts capable of oxidizing aqueous bisphenol A under visible light, Appl. Clay Sci., 2014, 93-94, 72–7710.1016/j.clay.2014.02.023Search in Google Scholar
 Raja R., Ratnasamy P., Selective oxidation of phenols using copper complexes encapsulated in zeolites, Appl. Catal. A-General, 1996, 143, 145–15810.1016/0926-860X(96)00077-4Search in Google Scholar
 Voronina A. A., Tarasyuk I. A., Marfin Y. S., Vashurin A. S., Rumyantsev E. V., Pukhovskaya S. G., Silica nanoparticles doped by cobalt(II) sulfosubstituted phthalocyanines: Sol–gel synthesis and catalytic activity, J. Non. Cryst. Solids, 2014, 406, 5–1010.1016/j.jnoncrysol.2014.09.009Search in Google Scholar
 Mirzaeian M., Rashidi A. M., Zare M., Ghabezi R., Lotfi R., Mercaptan removal from natural gas using carbon nanotube supported cobalt phthalocyanine nanocatalyst, J. Nat. Gas Sci. Eng., 2014, 18, 439–44510.1016/j.jngse.2014.03.023Search in Google Scholar
 Yao Y., Chen W., Lu S., Zhao B., Binuclear metallophthalocyanine supported on treated silk fibres as a novel air-purifying material, Dyes Pigments 2007, 73, 217–22310.1016/j.dyepig.2005.11.009Search in Google Scholar
 Rismayani S., Fukushima M., Sawada A., Ichikawa H., Tatsumi K., Effects of peat humic acids on the catalytic oxidation of pentachlorophenol using metalloporphyrins and metallophthalocyanines, J. Mol. Catal. A-Chem., 2004, 217, 13–1910.1016/j.molcata.2004.03.030Search in Google Scholar
 Wei Z., Cao Y., Ma W., Wang C., Xu W., Guo X., Hu W., Zhu, Langmuir–Blogett monolayer transistors of copper phthalocyanine, Appl. Phys. Lett., 2009, 95, 1–310.1063/1.3185151Search in Google Scholar
 Białek B., Kim I. G., Lee J. I., Electronic structure of copper phthalocyanine monolayer: a first-principles study, Thin Solid Films, 2003, 436, 107–11410.1016/S0040-6090(03)00521-2Search in Google Scholar
 Valkova L., Borovkov N., Pisani M., Rustichelli F., Structure of monolayers of copper tetra-(3-nitro-5-tert-butyl)-phthalocyanine at the air-water interface, Langmuir, 2001, 17, 3639–364210.1021/la0012079Search in Google Scholar
 Jiang Y., Lu Y., Lv X., Han D., Zhang Q., Niu L., Chen W., Enhanced catalytic performance of pt-free iron phthalocyanine by graphene support for efficient oxygen reduction reaction, ACS Catal., 2013, 3, 1263–127110.1021/cs4001927Search in Google Scholar
 Vargas E., Vargas R., Núñez O., A TiO2 surface modified with copper(II) phthalocyanine-tetrasulfonic acid tetrasodium salt as a catalyst during photoinduced dichlorvos mineralization by visible solar light, Appl. Catal. B Environ., 2014, 156-157, 8–1410.1016/j.apcatb.2014.02.045Search in Google Scholar
 Chen S., Huang X., Xu Z., Decoration of phthalocyanine on multiwalled carbon nanotubes/cellulose nanofibers nanocomposite for decoloration of dye wastewater, Compos. Sci. Technol., 2014, 101, 11–1610.1016/j.compscitech.2014.06.024Search in Google Scholar
 Vashurin A. S., Badaukaite R. A., Futerman N. A., Pukhovskaya S. G., Shaposhnikov G. P., Golubchikov O. A., Catalytic properties of polymer matrix-immobilized cobalt complexes with sulfonated phthalocyanines, Pet. Chem., 2013, 53, 197–20010.1134/S0965544113030122Search in Google Scholar
 Boury-Esnault N., Lavrov D. V., Ruiz C. A., Pérez T., The integrative taxonomic approach applied to porifera: A case study of the homoscleromorpha, Integr. Comp. Biol., 2013, 53, 416–42710.1093/icb/ict042Search in Google Scholar PubMed
 Ehrlich H., Maldonado M., Hanke T., Meissner H., Born R., Spongins: nanostructural investigations and development of biomimetic material model, VDI Berichte, 2003, 1843, 287–292Search in Google Scholar
 Pallela R., Bojja S., Janapala V. R., Biochemical and biophysical characterization of collagens of marine sponge, Ircinia fusca (Porifera: Demospongiae: Irciniidae), Int. J. Biol. Macromol., 2011, 49, 85–9210.1016/j.ijbiomac.2011.03.019Search in Google Scholar
 Green D., Howard D., Yang X., Kelly M., Oreffo R. O. C., Natural marine sponge fiber skeleton: a biomimetic scaffold for human osteoprogenitor cell attachment, growth, and differentiation, Tissue Eng., 2003, 9, 1159–116610.1089/10763270360728062Search in Google Scholar
 Ehrlich H., Biomimetic potential of chitin-based composite biomaterials of poriferan origin, In: Ruys A.J., Biomimetic biomaterials: structure and applications, Woodhead Publishing, 201310.1533/9780857098887.1.46Search in Google Scholar
 Szatkowski T., Wysokowski M., Lota G., Pęziak D., Bazhenov V. V., Nowaczyk G., Walter J., Molodtsov S. L., Stöcker H., Himcinschi C., Petrenko I., Stelling A. L., Jurga S., Jesionowski T., Ehrlich H., Novel nanostructured hematite-spongin composite developed using extreme biomimetic approach, RSC Adv. 2015, 5, 79031–7904010.1039/C5RA09379ASearch in Google Scholar
 Mahmoodi N. M., Salehi R., Arami M., Bahrami H., Dye removal from colored textile wastewater using chitosan in binary systems, Desalination, 2011, 267, 64–7210.1016/j.desal.2010.09.007Search in Google Scholar
 Rattanaphani S., Chairat M., Bremner J. B., Rattanaphani V., An adsorption and thermodynamic study of lac dyeing on cotton pretreated with chitosan, Dyes Pigments, 2007, 72, 88–9610.1016/j.dyepig.2005.08.002Search in Google Scholar
 Gómez J. M., Galán J., Rodríguez A., Walker G. M., Dye adsorption onto mesoporous materials: pH influence, kinetics and equilibrium in buffered and saline media, J. Environ. Manage., 2014, 146, 355–36110.1016/j.jenvman.2014.07.041Search in Google Scholar
 Pengthamkeerati P., Satapanajaru T., Singchan O., Sorption of reactive dye from aqueous solution on biomass fly ash, J. Hazard. Mater., 2008, 153, 1149–115610.1016/j.jhazmat.2007.09.074Search in Google Scholar
 Lagergren S., About the theory of so-called adsorption of soluble substances, Kungliga Svenska. Vetensk. Handl., 1898, 24, 1–39Search in Google Scholar
 Cook M. J., Cracknell S. J., Moore G. R., Osborne M. J., Williamson D. J., Solution phase 1H and 13C-NMR studies of some 1,4,8,11,15,18,22,25-octa-alkylphthalocyanines, Magn. Reson. Chem., 1991, 29, 1053–106010.1002/mrc.1260291014Search in Google Scholar
 Kaya E. Ç., Karadeniz H., Kantekin H., The synthesis and characterization of metal-free and metallophthalocyanine polymers by microwave irradiation containing diazadithia macrocyclic moieties, Dyes Pigments, 2010, 85, 177–18210.1016/j.dyepig.2009.10.021Search in Google Scholar
 Norman M., Bartczak P., Zdarta J., Tylus W., Szatkowski T., Stelling A., Ehrlich, H., Jesionowski T., Adsorption of C.I. Natural Red 4 onto spongin skeleton of marine demosponge, Materials, 2014, 8, 96–11610.3390/ma8010096Search in Google Scholar PubMed PubMed Central
 Kaušpėdienė D., Kazlauskienė E., Česūnienė R., Gefenienė A., Ragauskas R., Selskienė A., Removal of the phthalocyanine dye from acidic solutions using resins with the polystyrene divinylbenzene matrix, Chemija, 2013, 24, 171–181Search in Google Scholar
 Ueberlein S., Machill S., Niemann H., Proksch P., Brunner, The skeletal amino acid composition of the marine Demosponge Aplysina cavernicola, Mar. Drugs, 2014, 12, 4417–443810.3390/md12084417Search in Google Scholar PubMed PubMed Central
 Exposito J. Y., Garrone R., Characterization of a fibrillar collagen gene in sponges reveals the early evolutionary appearance of two collagen gene families, Proc. Natl. Acad. Sci. USA, 1990, 87, 6669–667310.1073/pnas.87.17.6669Search in Google Scholar PubMed PubMed Central
 Degirmencioglu I., Atalay E., Er M., Köysal Y., Işik Ş., Serbest K., Novel phthalocyanines containing substituted salicyclic hydrazone-1,3-thiazole moieties: microwave-assisted synthesis, spectroscopic characterization, X-ray structure and thermal characterization, Dyes Pigments, 2010, 84, 69–7810.1016/j.dyepig.2009.07.001Search in Google Scholar
 Ding L., Qiao J., Dai X., Zhang J., Zhang J., Tian B., Highly active electrocatalysts for oxygen reduction from carbon-supported copper-phthalocyanine synthesized by high temperature treatment, Int. J. Hydrogen Energy, 2012, 37, 14103–1411310.1016/j.ijhydene.2012.07.046Search in Google Scholar
 Agirtaş M. S., Gümüş I., Okumus V., Dundar A., Design of novel binuclear phthalocyanines formed by dioxyphenyl bridges: synthesis and investigation of thermal and antioxidant properties, Zeitschrift fur Anorg. und Allg. Chemie, 2012, 638, 1868–187210.1002/zaac.201200220Search in Google Scholar
 Pöhlker C., Huffmann J. A., Pöschl U., Autofluorescence of atmospheric bioaerosols – fluorescent biomolecules, biological standard particles and potential interferences, Geophys. Res. Abstr., 2012, 14, 110.5194/amt-5-37-2012Search in Google Scholar
 Pfannkuchen M., Schlesinger S., Fels A., Brümmer F., Microscopical techniques reveal the in situ microbial association inside Aplysina aerophoba, Nardo 1886 (Porifera, Demospongiae, Verongida) almost exclusively consists of cyanobacteria, J. Exp. Mar. Bio. Eco., 2010, 390, 169–17810.1016/j.jembe.2010.04.038Search in Google Scholar
 Wang X., Gao J., Xu B., Hua T., Xia H., ZnO nanorod/nickel phthalocyanine hierarchical hetero-nanostructures with superior visible light photocatalytic properties assisted by H2O2, RSC Adv., 2015, 5, 87233–8724010.1039/C5RA15821DSearch in Google Scholar
 Zhang M., Shao C., Guo Z., Zhang Z., Mu J., Cao T., Liu Y., Hierarchical nanostructures of copper(II) phthalocyanine on electrospun TiO2 nanofiber: controllable solvothermal- fabrication and enhanced visible photocatalytic properties, ACS Appl. Mater. Interfaces, 2011, 3, 369–37710.1021/am100989aSearch in Google Scholar
 Shang J., Zhao F., Zhu T., Li J., Photocatalytic degradation of rhodamine B by dye-sensitized TiO2 under visible-light irradiation, Sci. China Chem., 2011, 54, 167–17210.1007/s11426-010-4168-8Search in Google Scholar
 Ozoemena K., Kuznetsova N., Nyokong T., Comparative photosensitised transformation of polychlorophenols with different sulphonated metallophthalocyanine complexes in aqueous medium, J. Mol. Catal. A Chem., 2001, 176, 29–4010.1016/S1381-1169(01)00243-6Search in Google Scholar
 Yao G., Li J., Luo Y., Sun W., Efficient visible photodegradation of 4-nitrophenol in the presence of H2O2 by using a new copper(II) porphyrin-TiO2 photocatalyst, J. Mol. Catal. A Chem., 361-362, 29–3510.1016/j.molcata.2012.04.013Search in Google Scholar
 Poyatos J. M., Muñio M. M., Almecija M. C., Torres J. C., Hontoria E., Osorio F., Advanced oxidation processes for wastewater treatment: State of the art, Water Air Soil Pollut., 2010, 205, 187–20410.1007/s11270-009-0065-1Search in Google Scholar
 Pawlicki M., Kańska I., Latos-Grażyński L., Copper(II) and copper(III) complexes of pyrrole-appended oxacarbaporphyrin, Inorg. Chem., 2007, 46, 6575–658410.1021/ic700631tSearch in Google Scholar PubMed
 Wilhelm P., Stephan D., Photodegradation of rhodamine B in aqueous solution via SiO2@TiO2 nano-spheres, J. Photochem. Photobiol. A Chem., 2007, 185, 19–2510.1016/j.jphotochem.2006.05.003Search in Google Scholar
 Yu K., Yang S., He H., Sun C., Gu C., Ju Y., Visible light-driven photocatalytic degradation of rhodamine B over NaBiO3: Pathways and mechanism, J. Phys. Chem. A, 2009, 113, 10024–1003210.1021/jp905173eSearch in Google Scholar PubMed
 Luan J., Xu Y., Photophysical property and photocatalytic activity of new Gd2InSbO7 and Gd2FeSbO7 compounds under visible light irradiation, Int. J. Mol. Sci., 2013, 14, 999–102110.3390/ijms14010999Search in Google Scholar PubMed PubMed Central
 Mekprasart W., Vittayakorn N., Pecharapa W., Ball-milled CuPc/TiO2 hybrid nanocomposite and its photocatalytic degradation of aqueous Rhodamine B, Mater. Res. Bull., 2012, 47, 3114–311910.1016/j.materresbull.2012.08.024Search in Google Scholar
© 2016 Małgorzata Norman et al., published by De Gruyter Open.
This work is licensed under the Creative Commons Attribution-NonCommercial-NoDerivatives 3.0 License.